Kameyama et al.

Asian Pac J Dent 2019; 19: 51-57

Micrographic and spectroscopic analyses of the application of
methyl methacrylate-p-styrene sulfonic acid copolymer-baseddesensitizing agents to bovine dentin
Atsushi Kameyama, DDS, PhD (1,2), Akiko Haruyama, DDS, PhD (2), Yuichi Nakazawa,
DDS, PhD (2), Masahiro Furusawa, DDS, PhD (3), and Takashi Muramatsu, DDS, PhD(2)(1) Department of Operative Dentistry, Endodontology, and Periodontology, School of Dentistry,
Matsumoto Dental University, Shiojiri, (2) Department of Operative Dentistry, Cariology and Pulp
Biology, and (3) Department of Endodontics, Tokyo Dental College, Tokyo, Japan
Purpose: This study compared the ability of three methyl methacrylate (MMA)-p-styrene sulfonic acidcopolymer (MS polymer)-based desensitizers (Pain-Free Gel Dentin Desensitizer; PF-Gel, No-Mix Pain-Free
Desensitizer; PF, No-Mix Pain-Free F Desensitizer; PF-F) to occlude dentinal tubules.
Materials and Methods: Dentin disc specimens were prepared from bovine incisors and the desensitizers wereapplied. After dehydration for 24 h or immersion for 1 week in artificial saliva, the surfaces were observed byscanning electron microscope (SEM). PF-Gel specimens also underwent SEM/energy dispersive X-ray
spectroscopy (EDS).
Results: Application of the desensitizers produced complete occlusion of the dentinal tubules. Most dentinal
tubules re-opened after immersion for 1 week in artificial saliva (PF and PF-F samples), but in PF-Gel samples,the dentinal tubules remained occluded. SEM/EDS analysis demonstrated that the granular crystals adhering to
the dentin surface contained oxygen, carbon, and calcium, and the plugs occluding the dentinal tubules contained
calcium and phosphorus.
Conclusion: The findings in this study confirm the sustainable effect of PF-Gel on the occlusion of dentinal
tubules.
(Asian Pac J Dent 2019; 19: 51-57.)
Key Words: dentin desensitizer, dentinal hypersensitivity, MS polymer, energy dispersive X-ray spectroscopy

Introduction
Cervical dentin hypersensitivity, the most common cause of reversible dental pulpitis, is a common symptomaticcondition that causes discomfort in adult patients [1]. The clinical symptoms of cervical dentin hypersensitivity
are principally caused by exposure of dentinal tubules as a result of enamel loss and/or gingival root surface
exposure caused by gingival recession, abrasion, attrition, erosion, and abfraction [2,3]. Exposure of dentin withpatent dentinal tubules results in activation of A-delta pulpal nerve fiber endings, causing pain [4]. Several
hypotheses have been proposed to explain the mechanism of cervical dentin hypersensitivity. The hydrodynamic
theory proposed by Brännström [5,6] is the most generally accepted [7]. This theory suggests that
pain-provoking stimuli increase the movement of dentinal tubular fluid or change the flow direction, stimulating
A-delta pulpal nerve fibers around odontoblasts, and thereby leading to cervical dentin hypersensitivity.
Three main strategies have been introduced to treat cervical dentin hypersensitivity: 1) depolarization of thenerve by topical application of potassium nitrate (KNO3) [8]; 2) biological fixation of dentinal fluid bydenaturing protein using glutaraldehyde-containing desensitizer [9,10]; and 3) physical occlusion of the exposed
dentinal tubules [11]. Oxalate-containing products have been tested both in vitro [12-14] and in vivo [15,16].
Methyl methacrylate (MMA)-p-styrene sulfonic acid copolymer (MS polymer) is a water-soluble copolymer.
MS polymer cross-links with Ca2+ released from the tooth substrate and is immobilized on the tooth surface. MS
polymer-based desensitizers have been reported to seal the dentinal tubules and reduce hypersensitivity fromthermal, mechanical and chemical stimulation [17,18]. However, an MS polymer-based desensitizer containing

51

Kameyama et al.

Asian Pac J Dent 2019; 19: 51-57

1% oxalic acid (No-Mix Pain-Free, Sun Medical, Moriyama, Japan) has been reported to have lower tubule
occluding ability than a fluoro alumino calcium silicate-based desensitizer (Nanoseal, Nippon Shika Yakuhin,
Shimonoseki, Japan) and a calcium phosphate-based desensitizer (Teethmate Desensitizer, Kuraray Noritake
Dental, Tokyo, Japan) [13].
Recently, a modified MS polymer-based desensitizing agent was developed with the addition of a thickener toconvert it into gel form, with the aim of improving retention on the tooth surface. Strengthening of the dentin
and reduction of intra-dental nerve excitability could also be expected as a result of the addition of sodium
fluoride and potassium phosphate [18,19]. However, these effects have not yet been verified. The aim of this invitro study was therefore to investigate whether this newly developed MS polymer-based desensitizing gel could
increase the occlusion of the dentinal tubules. Also, changes in the tooth surface after immersion in artificial
saliva for 1 week were evaluated to investigate the sustainability of the dentinal tubule seal after application of
the MS polymer-based desensitizing gel.

Materials and Methods
Materials
Three MS polymer-based dentin desensitizers were used in this study; Pain-Free Gel Dentin Desensitizer (Sun
Medical), No-Mix Pain-Free Desensitizer (Sun Medical), and No-Mix Pain-Free F Desensitizer (Sun Medical)(Table 1).
Table 1 Materials used
Product (Manufacturer)

IngredientspH

Lot No.

Code

Pain-Free Gel Dentin Desensitizer*(Sun Medical, Moriyama, Japan)

MS polymer, 1% oxalic acid, water, sodium
fluoride (900 ppm F−), acidity regulator(potassium phosphate salt), thickener, others
MS polymer, 1% oxalic acid, water

2

LR11

PF-Gel

1.5

LL1

PF

2

MK1

PF-F

No-Mix Pain-Free** (Sun Medical)

No-Mix Pain-Free F Desensitizer***
MS polymer, 1% oxalic acid, water, sodium(Sun Medical)
fluoride (3,000 ppm F–)
MS polymer, methyl methacrylate (MMA)-p-styrene sulfonic acid copolymer*MS Coat Hys Block Gel, **MS Coat ONE, and ***MS Coat F, in Japan

Specimen preparation
Twelve extracted and non-damaged bovine incisors, frozen to maintain freshness, were defrosted, and theadherent soft tissue was removed under running tap water. They were cut at the enamel-dentin junction using a
low-speed diamond saw (Isomet, Buehler, Lake Bluff, IL, USA) and the pulp and soft tissue were removed. The
labial side of the enamel surface was abraded under a stream of water with #180 SiC paper to expose a flat
dentin surface. The specimens were sequentially abraded under a stream of water with #600 and #1,200 SiC
paper to form a 10 × 10 × 1 mm disc-shaped dentin specimen. The labial surface of the dentin specimens wasbrushed for 3 min using a manual toothbrush (Butler #411, Sunstar Suisse S.A., Etoy, Switzerland) andcommercial dentifrice (White & White, Lion, Tokyo, Japan), and ultrasonically cleaned in ultra-pure water for
35 min. Thereafter, these dentin specimens were sterilized in an autoclave (BS-245, Tomy, Tokyo, Japan) at
121˚C for 20 min.
Morphological analysis of the desensitizer-applied dentin
Seven dentin discs were divided into four groups (2 discs for PF-Gel, 2 discs for PF, 2 discs for PF-F, and 1 discfor non-applied control) for morphological analysis of the dentin. The discs were subjected to one of the52

Kameyama et al.

Asian Pac J Dent 2019; 19: 51-57

following treatments: PF-Gel, A rice grain-size amount of PF-Gel was applied to the dentin surface for 30 s, andthoroughly rinsed with running tap water; PF, One drop of PF was applied to the dentin surface for 120 s without
rubbing and dried with an air syringe; and PF-F, One drop of PF-F was applied to the dentin surface for 120 swithout rubbing and dried with an air syringe. The remaining dentin disc was used as a control.
The conditioned specimens were rinsed with running tap water and dried with air pressure. After dehydrationfor 24 h in a desiccator at room temperature, one specimen from each group was placed on an aluminum stuband Pt-coated using a super fine sputter coater (ESC-101, Elionix, Hachioji, Japan) for 120 s and examined
under scanning electron microscopy (SEM) (LSM-5610LV, JEOL, Akishima, Japan) at 3,500× magnification.
The other specimens were fractured longitudinally at the center with a cutting plier. They were placed on a stuband Pt-coated, and the cross-sectioned surface was examined under SEM at 8,000× magnification.
SEM analysis after 1-week immersion in artificial saliva
Three dentin discs were coated with PF-Gel, PF, or PF-F as for the morphological analysis of the dentin. The
specimens were immersed in 50 mL of artificial saliva (1.09 mmol/L CaCl2, 0.68 mmol/L KH2PO4, 30 mmol/L
KCl, 2.6 µmol/L NaF, 50 mmol/L HEPES; pH 7.0) at 37˚C for 7 days [20]. The immersing solution waschanged every 24 h. Each specimen was then rinsed with ultra-pure water and dried with air pressure. Afterdehydration for 24 h in a desiccator at room temperature, they were placed on an aluminum stub, Pt-coated andexamined under SEM.
Energy dispersive X-ray spectroscopy (EDS) analyses of PF-Gel specimens
The remained two dentin discs were coated with PF-Gel, and one was immersed in 50 mL of artificial saliva inthe same manner (37˚C for 7 days). These specimens were cleaned, air-dried, and dehydrated for 24 h. Eachspecimen was osmium-coated for 10 s (7 Pa of vacuum, 10 mA) using osmium coater (Neoc-STB, Meiwafosis,
Tokyo, Japan) and analyzed at a decomposition depth of about 100 nm under high-resolution SEM/EDS (S-4800,
Hitachi High-Technologies, Tokyo, Japan / Quantex Flat Quad, Bruker, Yokohama, Japan) at 6 kV.

Results
Morphological analysis of the desensitizer-applied dentin
Figure 1 demonstrates SEM images of the dentin surface and longitudinal cross-section in each group that did
not undergo the 1-week immersion in artificial saliva. The control specimen (not treated with any desensitizer)
confirmed the absence of a smear layer on the dentin surface because scratches caused by abrasion with the SiC
paper could be clearly detected (Fig. 1d, black arrow). Open dentinal tubules were all clearly visible (Fig. 1d). In
contrast, complete occlusion of the dentinal tubules was seen after treatment with any of the MS polymer-baseddesensitizing agents (Fig. 1a-c). Globular-like deposits could also be detected on the dentin surface and within
the dentinal tubules. Sagittal views showed that the dentin surface was completely covered with a thin layer ofdesensitizer which appeared to completely occlude the dentinal tubules in all PF-Gel, PF and PF-F specimens(Fig. 1e-g).
Figure 2 shows SEM images of the dentin surfaces in each group after a 1-week immersion in artificial saliva.
PF-Gel specimens were still covered with globular-like deposits on the dentin surface and within the dentinal
tubules, and no open dentinal tubules were detected (Fig. 2a). However, almost all dentinal tubules were open in
PF and PF-F specimens (Fig. 2a,b).

53

Kameyama et al.

Asian Pac J Dent 2019; 19: 51-57

Fig. 1 Scanning electron micrographs showing the dentin surface (original magnification 3,500x) and longitudinal fractures(original magnification 8,000x) after application of MS polymer-based desensitizers; PF-Gel (a, e), PF (b, f), PF-F (c, g),and the control dentin surface (no desensitizer applied) (d). Globular-like deposits can be seen on the treated dentin
surface and within the dentinal tubules. The dentin surface is completely covered with a thin layer of desensitizer whichappears to completely occlude the dentinal tubules (pointers). The control dentin surface shows scratches caused byabrasion with SiC paper (black arrow), and the dentinal tubules are all open. Bar scale 2 µm.

Fig. 2 Scanning electron micrographs of the dentin surface after application of MS polymer-based desensitizers followed byimmersion for 1 week in artificial saliva (original magnification 3,500x); PF-Gel (a), PF (b), and PF-F (c). Some dentinal
tubules are open in PF and PF-F specimens (open arrows). However, dentinal tubules remain sealed in the PF-Gel
specimens after immersion for 1 week in artificial saliva (white arrowheads). Bar scale 5 µm.

Fig. 3 Scanning electron microscopy/energy dispersive X-ray spectroscopy (SEM/EDS) mapping images of the dentin surfacesof PF-Gel specimens (original magnification 5,000x). After application of PF-Gel, granular crystals can be seen adheringto the dentin surface, and oxygen (O), carbon (C) and calcium (Ca) are present. The plugs of the dentinal tubules show
the presence of Ca and phosphorus (P). Fluorine (F) can be detected locally around the dentinal tubules. After immersion
in artificial saliva for 1 week, granular deposits can be seen on the dentin surface. Although Ca and O have diminishedaround the intertubular dentin, C is retained. The plugs of the dentinal tubules show the presence of Ca and P, and F canbe detected over the entire dentin surface. Bar scale 5 µm.

54Kameyama et al.

Asian Pac J Dent 2019; 19: 51-57

EDS analyses of PF-Gel specimens
Figure 3 shows the mapped surfaces of the dentin coated with PF-Gel under SEM/EDS analysis. The specimens
examined immediately after coating showed granular crystals containing oxygen, carbon and calcium adheringto the dentin surface (Fig. 3b,c,e). The plugs in the dentinal tubules showed the presence of calcium andphosphorus (Fig. 3d,e). Fluorine was detected around the dentinal tubules (Fig. 3f). The specimens immersed for
1 week in artificial saliva exhibited smaller and fewer granular deposits on the dentin surface. The plugs in thedentinal tubules showed the presence of calcium and phosphorus (Fig. 3j,k). Fluorine was detected over theentire dentin surface (Fig. 3l).

Discussion
PF has a relatively strong demineralization effect because of its strong acidity (pH 1.5). When MS polymer isapplied to the dentin surface, it can react with Ca2+ ions supplied by demineralized hydroxyapatite from thesmear layer, producing an MS polymer-Ca complex and covering the exposed dentin surface. Soluble oxalate
salts have been known to form and deposit slightly soluble calcium oxalate (CaC2O4) crystals on the dentin
surface by binding with Ca2+ ions from the smear layer [21-23]. Therefore, it was thought that application ofoxalic acid-containing MS polymer-based desensitizer would result in occlusion of the dentinal tubules by the
MS polymer-Ca complex and CaC2O4 crystals, thereby reducing the permeability of the dentinal tubules, andcontributing to the prevention of dentin hypersensitivity [16]. The present findings confirming that the dentinal
tubules are completely occluded immediately after applying PF support previous studies that demonstrated an
immediate reduction in dentin permeability after application of an oxalic acid-containing MS polymer-baseddesensitizer [14,24].
PF-F contains sodium fluoride in the aqueous solution. Although fluoride ions do not contribute directly totubular occlusion, acidic fluoride varnishes have been reported to react with dentin to release Ca2+ that can form
calcium fluoride (CaF2) with the varnish base; these CaF2 particles can migrate into and occlude the dentinal
tubules [25]. Oshima et al. recently reported that PF-F-treated dentin showed significantly lower mineral loss
than PF-treated dentin after acidic challenge (5 h, pH 4.5) [18]. They also observed a 2-3 µm-thick layer-likestructure covering the dentin surface and the dentinal tubules even after the acidic challenge. Therefore, PF-F isexpected to not only prevent dentin hypersensitivity, but also prevent root dentin demineralization.
The results of our study and other previous studies showed that oxalate salts are effective in producing
calcium oxalate crystals on the dentin surface. However, calcium oxalate crystals have been reported to either
partially dissolve in saliva or oral fluids, or disappear during toothbrushing [15,20,23,26,27]. Therefore, thesustainability of the MS polymer-based desensitizing agents on the occlusion of dentinal tubules after immersion
in artificial saliva also was evaluated. The present results support the previous reports [27] that found thatcalcium oxalate crystals dissolved on the dentin surface and the dentinal tubules were open in both PF and PF-F
specimens. Therefore, in the clinical situation, it is recommended to apply them repeatedly at each visit.
Although the PF-Gel-coated dentin surface was covered with a granular precipitate in the same way as the PF
and PF-F specimens, the granules were larger and denser than those of the PF and PF-F specimens. Because
SEM/EDS evaluation detected that the granular crystals were composed of O, C, and Ca, it was presumed thatthey were crystals of calcium oxalate. Additionally, the localization of phosphorus and calcium observed aroundthe dentinal tubules suggests the formation of calcium phosphate or its fluoride (calcium fluoride). Therefore,

55

Kameyama et al.

Asian Pac J Dent 2019; 19: 51-57

thickeners added to the PF-Gel may have helped to retain the MS polymer and oxalic acid on the tooth surface[31], thereby efficiently promoting the formation of calcium oxalate, calcium phosphate, and calcium fluoride
crystals.
In contrast with the PF and PF-F specimens, the dentinal tubules of the PF-Gel specimens remainedcompletely closed even after a 1-week immersion in artificial saliva. Additionally, the granular crystals remainedon the dentin surface, although they were smaller than those in the immediate specimen. Varoni et al. recently
demonstrated the effect of a novel potassium oxalate hydrogel in reducing the solubility of potassium oxalate
crystals, and thereby improving the efficacy of potassium oxalate as a dentinal tubule-occluding agent [32]. They
presumed that the time-dependent occlusive effect on dentinal tubules is probably a result of the presence of theactive ingredient, rather than a direct effect of the hydrogel itself. Our results supported their presumption.
Therefore, the thickeners in PF-Gel may also have reduced the solubility of the calcium oxalate crystals andallowed the resin-based component (MS polymer) to be retained.
Localized calcium and phosphorus were also detected at the plugged dentinal tubules, and deposits of fluorine
were detected over the entire dentin surface after immersion for 1 week in artificial saliva. Therefore, the crystals
occluding the dentinal tubules could be calcium phosphate and calcium fluorophosphates Ca5(PO4)3F. Formationof these crystals may not only suppress the penetration into the dentinal tubule, but may also inhibit thedemineralization of exposed root dentin in the same way as PF-F [18]. PF-Gel contains potassium phosphate as a
pH adjuster, and this component may also contribute a nerve-numbing effect caused by the potassium ions
[8,29].
Acknowledgments
This work was partially supported by JSPS KAKENHI Grant Numbers JP 17K11715 and JP 16K20464.
Conflicts of Interest
The authors declare that there are no conflicts of interest regarding the publication of this paper.

References
1.
2.
3.
4.
5.
6.
7.
8.
9.
10.
11.
12.
13.
14.
15.
16.
17.
18.

Brännström M. The elicitation of pain in human dentine and pulp by chemical stimuli. Arch Oral Biol 1962; 7: 59-62.
Addy M, Dowell P. Dentine hypersensitivity – a review. Clinical and in vitro evaluation of treatment agents. J Clin Periodontol
1983; 10: 351-63.
Pashley DH. Mechanisms of dentin sensitivity. Dent Clin North Am 1990; 34: 449-73.
Pashley DH. Dentine permeability and its role in the pathobiology of dentine sensitivity. Arch Oral Biol 1994; 39 Suppl:
73S-80S.
Brännström M. The hydrodynamic theory of dentinal pain: sensation in preparations, caries, and the dentinal crack
syndrome. J Endod 1986; 12: 453-7.
Brännström M, Aström A. A study of the mechanism of pain elicited from the dentin. J Dent Res 1964; 43: 619-25.
Gillam DG. Mechanisms of stimulus transmission across dentine. A review. J West Soc Periodontol Periodontal Abstr 1995;
43: 53-65.
Hodosh M. A superior desensitizer – potassium nitrate. J Am Dent Assoc 1974; 88: 831-2.
Schüpbach P, Lutz F, Finger WJ. Closing of dentinal tubules by Gluma desensitizer. Eur J Oral Sci 1997; 105(5Pt1): 414-21.
Qin CY, Xu J, Zhang Y. Spectroscopic investigation of the function of aqueous 2-hydroxyethylmethacrylate/glutaraldehyde
solution as a dentin desensitizer. Eur J Oral Sci 2006; 114: 354-9.
Mantzourani M, Sharma D. Dentine sensitivity: Past, present and future. J Dent 2013; 41(S4): S3-S17.
Zhang Y, Agee K, Pashley DH, Pashley EL. The effects of Pain-Free Desensitizer on dentine permeability and tubule
occlusion over time, in vitro. J Clin Periodontol 1998; 25(11Pt1): 884-91.
Gillam DG, Mordan NJ, Sinodinou AD, Tang JY, Knowles JC. The effects of oxalate-containing products on the exposed
dentine surface: an SEM investigation. J Oral Rehabil 2001; 28: 1037-44.
Han L, Okiji T. Dentin tubule occluding ability of dentin desensitizers. Am J Dent 2015; 28: 90-4.
Gillam DG, Coventry JF, Manning RH, Newman HN, Bulman JS. Comparison of two desensitizing agents for the treatmentof cervical dentine sensitivity. Endod Dent Traumatol 1997; 13: 36-9.
Erdemir U, Yildiz E, Kilic I, Yucel T, Ozel S. The efficacy of three desensitizing agents used to treat dentin hypersensitivity. J
Am Dent Assoc 2010; 141: 285-96.
Dall'Orologio GD, Ishihata H, Finger WJ, Sasaki K. In vitro and in vivo evaluation of the effectiveness of three dentin
desensitizing treatment regimens. Am J Dent 2014; 27: 139-44.
Oshima M, Hamba H, Sadr A, Nikaido T, Tagami J. Effect of polymer-based desensitizer with sodium fluoride on preventionof root dentin demineralization. Am J Dent 2015; 28: 123-27.

56

Kameyama et al.

Asian Pac J Dent 2019; 19: 51-57

19. Ma Q, Wang T, Meng Q, Xu X, Wu H, Xu D, et al. Comparison of in vitro dentinal tubule occluding efficacy of two different
methods using a nano-scaled bioactive glass-containing desensitising agent. J Dent 2017; 60: 63-9.
20. Suge T, Ishikawa K, Kawasaki A, Yoshiyama M, Asaoka K, Ebisu S. Duration of dentinal tubule occlusion formed by calcium
phosphate precipitation method: In vitro evaluation using synthetic saliva. J Dent Res 1995; 74: 1709-14.
21. Pashley DH, Carvalho RM, Pereira JC, Villanueva R, Tay FR. The use of oxalate to reduce dentin permeability underadhesive restorations. Am J Dent 2001; 14: 89-94.
22. Pereira JC, Segala AD, Gillam DG. Effect of desensitizing agents on the hydraulic conductance of human dentin subjected
to different surface pre-treatments - an in vitro study. Dent Mater 2005; 21: 129-38.
23. de Andrade e Silva SM, Marquezini L Jr, Manso AP, Garcia FP, Carrilho MR, Pashley DH, et al. Effects of a combined
application of potassium oxalate gel/adhesive agent on dentin permeability in vitro. J Adhes Dent 2007; 9: 505-12.
24. Ishihata H, Kanehira M, Nagai T, Finger WJ, Shimauchi H, Komatsu M. Effect of desensitizing agents on dentin permealibity.
Am J Dent 2009; 22: 143-6.
25. Arends J, Duschner H, Ruben JL. Penetration of varnishes into demineralized root dentine in vitro. Caries Res 1997; 31:
201-5.
26. Gillam DG, Newman HN, Davies EH, Bulman JS, Troullos ES, Curro FA. Clinical evaluation of ferric oxalate in relieving
dentine hypersensitivity. J Oral Rehabil 2004; 31: 245-50.
27. Balevi B. Oxalates may not be effective in treating dentin hypersensitivity. J Am Dent Assoc 2012; 143: 614-5.
28. Varoni EM, Zuccheri T, Carletta A, Palazzo B, Cochis A, Colonna M, et al. In vitro efficacy of a novel potassium oxalatehydrogel for dentin hypersensitivity. Eur J Oral Sci 2017; 125: 151-9.
29. Wanachantararak S, Vongsavan N, Matthews B. Electrophysiological observations on the effects of potassium ions on the
response of intradental nerves to dentinal tubular flow in the cat. Arch Oral Biol 2011; 56: 294-305.

Correspondence to:
Dr. Atsushi Kameyama
Department of Operative Dentistry, Endodontology, and Periodontology,
School of Dentistry, Matsumoto Dental University
1780 Gobara Hirooka, Shiojiri 399-0781, Japan
Fax: +81-263-51-2026, E-mail: atsushi.kameyama@mdu.ac.jp
Copyright ©2019 by the Asian Pacific Journal of Dentistry.

57

Accepted June 5, 2019.
Online ISSN 2185-3487, Print ISSN 2185-3479